The efficiency of Fenton-like catalysis using nano zerovalent iron (nZVI) is limited by nZVI aggregation and activity loss due to inactive ferric oxide forming on the nZVI surface, which hinders electron transfer. A novel iron–carbon composite catalyst consisting of nZVI and granular activated carbon (GAC), which can undergo internal iron–carbon microelectrolysis spontaneously, was successfully fabricated by the adsorption–reduction method. The catalyst efficiency was evaluated in nitrobenzene (NB) removal via the Fenton-like process (H2O2-nZVI/GAC). The results showed that nZVI/GAC composite was good for dispersing nZVI on the surface of GAC, which permitted much better removal efficiency (93.0%) than nZVI (31.0%) or GAC (20.0%) alone. Moreover, iron leaching decreased from 1.28 to 0.58 mg/L after reaction of 240 min and the oxidation kinetic of the Fenton-like reaction can be described well by the second-order reaction kinetic model (R2 = 0.988). The composite catalyst showed sustainable catalytic ability and GAC performed as a medium for electron transfer in internal iron–carbon microelectrolysis to promote Fe2+ regeneration and Fe3+/Fe2+ cycles. Therefore, this study represents an important method to design a low cost and high efficiency Fenton-like catalyst in practical application.
Nitrobenzene (NB) is deemed a priority control pollutant by the US Environmental Protection Agency (EPA) and other countries due to its high chemical stability, low biodegradability, and high toxicity (Roy et al. 2013). To date, a range of chemical and biological methods have been developed for aqueous NB treatment, such as advanced oxidation process (AOPs), microelectrolysis, and biological anaerobic process (Patil et al. 2011; Wang et al. 2011). As one of the important AOPs, the Fenton reaction has a good prospect for NB treatment because of the advantages of high mineralization efficiency, easy implementation, and cost saving (Bokare & Choi 2014). Recently, nano zerovalent iron (nZVI, Fe0) has been reported to be more effective in activation of hydrogen peroxide (H2O2) to generate hydroxyl radicals (•OH) than classified soluble ferrous ions (Fe2+) in the Fenton-like process (Fu et al. 2014). Nevertheless, nZVI as a Fenton-like catalyst is limited because of Fe2+ regeneration difficulty and activity loss due to inactive ferric oxides forming on the nZVI surface. In addition, lack of stability, easy aggregation, and difficult separation from treated solution are problems of nZVI use in actual application (Messele et al. 2014).
Activated carbon (AC) as a support has been proved to be effective for increasing dispersion and impeding aggregation of metallic nanoparticles (Xiao et al. 2014). Recently, many studies have indicated that an iron–carbon microelectrolysis system can be formed between AC and iron spontaneously when iron (anode) and AC (cathode) particles are mixed and contact with each other (Dou et al. 2010; Mackenzie et al. 2012; Luo et al. 2014). The activity of the Fenton-like reaction enhanced by iron–carbon microelectrolysis to remove dyes (Yao et al. 2013; Singh et al. 2014; Sun et al. 2014), trichloroethylene (Su et al. 2013), ionic liquids (Zhou et al. 2013), Cr(VI) (Wu et al. 2013), etc. have been investigated through combining Fe0 or common iron powder with AC. These results revealed that catalytic oxidation efficiency of the Fenton-like catalyst was significantly intensified when carbon was involved in the catalyst. This phenomenon can be explained by the internal iron–carbon microelectrolysis effect that exists in such an iron-AC combination system where AC acts as a migration medium for electrons, accelerating in situ regeneration of Fe2+ (Su et al. 2013; Singh et al. 2014; Sun et al. 2014). Thus, the fast cycle of Fe3+ and Fe2+ on AC surface will provide continuous Fe2+ to catalyze H2O2 to generate active •OH, which is a great potential advantage for practical NB wastewater treatment. In addition, it has been confirmed that AC is a good Fenton catalyst for NB degradation (Tan et al. 2013).
As far as we know, the Fenton-like catalysis using a composite of nZVI and AC for NB removal has not been investigated up to now. Moreover, AC is often used in the form of granular activated carbon (GAC), which is the most widely used adsorbent for water treatment. Therefore, nZVI/GAC composite was prepared by adsorption–liquid phase reduction, and its performance for NB removal from aqueous solution was evaluated by the Fenton-like system (H2O2-nZVI/GAC), with the aim of exploring a novel heterogeneous Fenton-like catalyst for refractory organic wastewater treatment in a cost-effective way.
MATERIALS AND METHODS
GAC derived from biomass was purchased from Gongyi Tongxin Water Treatment Material Co., Ltd (Henan, China). Before use, the GAC was soaked in 1 M HNO3 for 24 h followed by repeated rinsing with deionized water (resistance > 18 MΩ) and then dried at 105 °C. Other reagents used in this study were purchased from the Xi'an Chemical Corporation (Xi'an, China) and were of analytical grade.
Preparation of nZVI/GAC composite
After reduction, the black solids were separated from the solution using a vacuum filtration flask (0.45 μm membrane filter) and washed several times with degassed deionized water to remove residual sulfate, then vacuum-dried at 60 °C and stored in a N2-purged desiccator. Unsupported nZVI particles were also prepared in a similar way without GAC, and in all syntheses, N2 was bubbled into solution during the entire process to maintain an inert atmosphere. The nZVI loaded amount on GAC was 64.3 μmol/g calculated according to the procedure reported by Zhu et al. (2009).
The model wastewater was prepared by dissolving NB (>99%) in deionized water with final concentration of 40 mg/L. Then, 200 mL of wastewater was placed in a 250-mL brown flask and pH values were adjusted to 3.0, 4.0, and 5.0 with 1 M H2SO4. The dosages of 0.2, 0.4, and 0.6 g/L nZVI/GAC and 2.5, 5.0, and 10.0 mmol/L H2O2 solutions were added according to the designed Fe2+ and H2O2 molar ratio, and the initial dissolved oxygen of the mixed solution was 7.24 mg/L. The flask was capped and stirred on a thermostatic magnetic stirrer at 300 rpm with temperature of 25 °C and sampled regularly with intervening time of 15 or 30 min. The dosages of bare nZVI and GAC were equivalent to that in the nZVI/GAC composite, which were determined by nZVI loading in the composite. All experiments were conducted in triplicate and analysis showed that relative errors were lower than ±5%.
Scanning electron microscopy (SEM) (Vega 3 LMH, Tescan, Czekh) was used to view the morphology and surface characteristics of nZVI/GAC composite. The NB concentrations were determined using a high-performance liquid chromatograph equipped with a Waters symmetry C-18 column (150 mm × 4.6 mm i.d., 5 μm). The mobile phase was a mixture of methanol and 5 mM H3PO4 in the ratio of 3:2 (v/v) (isocratic). The flow rate was set at 1 mL/min and detection wavelength was set to 267.5 nm, and the column temperature was maintained at 25 °C. The samples were filtered through 0.45 μm filters and then 20 μL was injected manually through an injection port. All the prepared samples were taken for analysis immediately.
RESULTS AND DISCUSSION
The morphology of nZVI/GAC composite
Enhancement of nZVI/GAC composite as Fenton-like catalyst for NB removal
Furthermore, dissolved iron was monitored for both nZVI and nZVI/GAC composite as a Fenton-like catalyst (Figure 2(c)). For the composite, dissolved iron was <0.6 mg/L; by comparison with nZVI, the amount was reduced to half (from 1.28 to 0.58 mg/L) (Figure 2(c)), indicating that iron utilization efficiency was obviously raised and iron leaching was reduced because of the high adsorption capacity of GAC in the Fenton-like reaction.
Effect of nZVI/GAC composite dosages on Fenton-like NB removal
Effect of hydrogen peroxide concentrations on Fenton-like NB removal
Effect of initial pH values on Fenton-like NB removal
According to previous research, pH value is an important reaction parameter affecting Fenton removal of NB (Bokare & Choi 2014). An optimum working pH range is 2.8–3.2 for classical Fenton reaction, and widening the pH range is required for practical application (Bokare & Choi 2014; Fu et al. 2014). Thus, typical experiments at pH 3.0, 4.0 and 5.0 were carried out individually to check the extent of Fenton-like removal efficiency with nZVI/GAC composite as the catalyst.
Figure 5 also implies that the best degradation of NB was attained at pH 4.0 and the composite will still have activity at pH over 4.0. This conclusion was remarkably well supported by the result that NB removal ratio was 86.0% at pH 5.0. This is an important advantage because it is well known that one major drawback of the homogeneous Fenton process is the narrow pH range (pH < 3.0) (Pignatello et al. 2006), because such a narrow pH range is unfavorable in practice due to the costs of acidification during processing and neutralization after treatment. The possible mechanisms are that, with the involvement of GAC, Fenton oxidation occurs mostly on the interface of the nZVI/GAC composite, and continuous regeneration of Fe2+ is accelerated by internal microelectrolysis, and thus, inactive ferric oxide formation is reduced, mitigating the pH-limited reaction of conventional Fenton, and it may be feasible to use a wider pH range above pH 5.0. For these reasons, further experiments will be carried out at pH over 5.0 using the promising composite catalyst for refractory organic degradation.
The involvement of GAC greatly improved the dispersion of nZVI and dramatically intensified NB removal with nZVI/GAC composite as Fenton-like catalyst. NB removal efficiency increased from 31.0% for nZVI alone to 93.0% for nZVI/GAC composite after reaction of 240 min, and dissolved iron decreased from >1.2 mg/L to <0.6 mg/L. Not only was the Fenton-like catalysis using nZVI/GAC composite a good combination of adsorption by GAC and Fenton oxidation by nZVI, but also some synergetic effects existed in such a composite, because GAC in the composite performed as an electron transfer medium for internal iron–carbon microelectrolysis to enhance Fe3+/Fe2+ cycles. Therefore, although used in limited pH range, this novel composite represents an important step in the development of new inexpensive and efficient materials to remove refractory organics by the Fenton-like method, and of course the mechanism and influencing factors need to be thoroughly researched in further studies.
The project was financially supported by the National Natural Science Foundation of China (Grant No. 40872164, 41502240), fund for basic research from the Northwestern Polytechnical University (No. JCY20130145), China geological survey project (12120114056201), and graduate starting seed fund of Northwestern Polytechnical University (Z2015147).